Share this document with a friend

44

Transcript

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 1

Spontaneous time-reversal symmetry breaking (TRSB) in superconductors

and related materials

Department of Physics, CMTC, JQIUniversity of Maryland, College Park, USA

Victor Yakovenko

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Faraday effect:Polarization rotation of transmitted light

Kerr effect:Polarization rotation of reflected light

Faraday and Kerr effects in a magnetic field

2

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Circular dichroism

Right and left circularly-polarized modes have different refraction indices due to Hall conductivity:

Kerr effect was observed in the PG phase of cuprates by Kapitulnik since 2008, interpreted as time-reversal symmetry breaking (TRSB).

Faraday rotation

Kerr rotation(requires dissipation)

3

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Fried et al, Rev Sci Instr 85, 103707 (2014)4

Ultrasensitive apparatus for optical detection of time-reversal symmetry breaking

10 m fiber

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 5

Xia, …, Kapitulnik, PRL 97, 167002 (2006)

Polar Kerr effect and TRSB in Sr2RuO4

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 6

Schemm, …, Kapitulnik, Science 345, 190 (2014)

Polar Kerr effect and TRSB in UPt3

Two superconducting transitions

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 7

Schemm, …, Kapitulnik, PRB 91, 140506 (2015)

Polar Kerr effect and TRSB in URu2Si2

Hidden order THO=17.5 K

Super-conductivity Tc=1.5 K

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 8

Theory of the high-frequency chiral optical response of a px+ipy superconductor

Victor Yakovenko with Roman Lutchyn and Pavel Nagornykh

PRL 98, 087003 (2007) PRB 77, 144516 (2008) PRB 80, 104508 (2009)

Joint Quantum Institute (JQI) at the University of Maryland

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 9

The experiment shows that the superconducting order parameter in Sr2RuO4 must have intrinsic vorticity. The natural candidate is the triplet px+ipy pairing (Rice & Sigrist, 1995):

px

pϑp Δ(p) accumulates phase 2π

around the Fermi surface – a vortex in momentum space.

Kerr rotation is permitted by symmetry in this case, but we need to calculate the magnitude of the Kerr angle θK.

The experiment gives θK = 65 nanorad at T=0.

It represents the Cooper pairing between electrons with a non-zero angular momentum Lz=1.

�

ψ p( )ψ −p( ) ∝Δ p( ) = Δ 0 px + ipy( ) / pF = Δ 0eiϑ p

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 10

where n is the refraction coefficient, d is the interlayer distance.

The ac Hall conductivity σxy(ω) can be obtained by calculating the one-loop current-current response function

Ax Ay

According to the textbook,

using the Nambu Green function for a chiral superconductor

( )( )

3 1 22 2

ˆ ˆ ˆx x y yi p pG

Eω ε τ τ τ

ω

+ + Δ −Δ= −

+

pp

However, this diagram vanishes identically (by taking traces, before integration), even though it is permitted by symmetry.

�

θK = Im4πσ xy ω( )n n2 −1( )ωd

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 11

On the other hand, the one-loop current-charge response function does not vanish for a chiral superconductor

Ax,y A0

It was calculated by Volovik (JETP 1988) for ω=0 (dc response) and by Yakovenko (PRL 2007) for ω≠0 (ac response).

It describes a change of the electron charge density ρ in response to an applied magnetic field Bz:

This diagram generates the Chern-Simons-like term in the effective action of the system:

( )( )0 / 2 / ,xy t y x x yS dxdydt A e A A cσ ϕ= + ∂ ∂ − ∂∫

�

ρ = δSδA0

= 12e2

hcBz

where φ is the superconducting phase.

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 12

However, the anomalous charge response does not imply the Hall effect. The Štreda formula does not apply to superconductors!

The effective action gives the Hall-like current

The electric charge of a standard vortex with the flux quantum ϕ0=hc/2e is Q=e/4 (Goryo 2000, Stone & Roy 2004).

Magnetoelectric response

Proposed experiment to detect electric charge induced by magnetic field (Lutchyn, Nagornykh, Yakovenko 2008)

�

j = c δSδA

=σ xy E − 12e

∂∂t ∇ϕ − 2e

c A( )[ ]× ˆ z

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 13

When the effective action for the superconducting phase φ is added, and φ is integrated out, the Hall current vanishes ▪Goryo and Ishikawa, Phys. Lett. A 1998, 1999 ▪Horovitz and Golub, Europhys Lett 2002, PRB 2003 ▪Lutchyn, Nagornykh, and Yakovenko, PRB 2008 ▪Roy and Kallin, PRB 2008

Vanishing of the Hall current for a chiral superconductor can be understood as a consequence of the Galileo invariance (Read and Green, PRB 2000). In the absence of an external magnetic field, an electric field cannot cause a sideways deflection of an electron cloud, even if electrons have the chiral Cooper pairing.

So, the only way to produce a non-zero Hall effect in a chiral superconductor is by taking into account impurity scattering. It produces “friction” between the Cooper pairs and the lattice, which results in a sideways Magnus force.

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 14

However, the lowest-order diagram with one impurity line vanishes identically (by taking traces):

Ax Ay

A non-zero Hall effect comes from the following diagrams:

Ax Ay

Goryo PRB 2008: In this diagram, the sign of the Hall effect is determined by the sign of the impurity potential.

Lutchyn, Nagornykh, Yakovenko, PRB 80, 104508 (2009): The Hall effect sign depends on the electron-hole asymmetry.

Ax Ay Ax Ay

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 15

Goryo’s diagram for σxy(ω) (non-Gaussian disorder)

Divergence

�

1ω − 2Δ 0

at ω → 2Δ 0

For ω>>Δ0:

�

σ xy(3) ω( ) = − e

2

!WΔ 0

ω 3 i + 4πΔ 0

ωln ω

Δ 0

⎛

⎝ ⎜

⎞

⎠ ⎟

⎡

⎣ ⎢

⎤

⎦ ⎥ at T = 0

σ xy(3) ω( ) = − e

2

!WΔ 0

ω 3Δ 0

Tci2

+ 4πTcωln ω

Tc

⎛

⎝ ⎜

⎞

⎠ ⎟

⎡

⎣ ⎢

⎤

⎦ ⎥ at T→ Tc

�

σ xy(3) ω = 0( ) = 8

105πe2

!WΔ02

General property: σ(ω)=σ*(-ω)

Red – imaginary, blue – real part

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 16

Temperature dependence of the high-frequency σxy(ω) (for non-Gaussian disorder)

�

′ ′ σ xy(3) ω,T( )′ ′ σ xy(3) ω,0( )

= Δ 0(T)Δ 0(0)

tanh Δ 0(T)2T

⎛ ⎝ ⎜

⎞ ⎠ ⎟

for ω >> Tc

�

σ xy ∝Δ xΔ y ∝Δ 02 T( ) ∝ Tc −T( )For T near Tc, we find

Our theory: PRB 80, 104508 (2009)

Experimental data: Kapitulnik et al., New J Phys 11, 055060 (2009)

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 17

Anomalous σxy(ω) for multi-band superconductivity▪Taylor and Kallin, PRL 108, 157001 (2012); J Phys Conf

Ser 449 012036 (2013), 3-band model for Sr2RuO4 ▪Gradhand, Wysokiński, Annett, Györffy, PRL 108, 077004

(2012); PRB 88, 094504 (2013); J Phys Cond Mat 26 274205 (2014); Phil Mag 95, 525 (2015) ▪Brydon and Yakovenko, in preparation, 2-band

superconducting pairing on a hexagonal lattice for TMD

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 18

Conclusions

▪The Hall effect for a clean one-band chiral superconductor (without impurities) vanishes identically. ▪A non-zero Hall effect can be obtained only if we take into

account impurity scattering or multi-band superconductivity. ▪Magnitude of the Hall effect depends on the concentration

of impurities and strength of the scattering potential. ▪There is a preliminary experimental indication that the Kerr

effect is stronger in the Sr2RuO4 samples of the lower quality, i.e. with the higher concentration of defects. ▪Temperature dependence of the Kerr angle follows θK~Δ2(T)~(Tc−T) neat Tc.

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 19

Connection with the quantum field theory

“Pseudogap and time reversal breaking in a holographic superconductor” M. M. Roberts and S. A. Hartnoll Journal of High-Energy Physics 8, 035 (2008)

Abstract: Classical SU(2) Yang-Mills theory in 3+1 dimensional anti-de Sitter space is known to provide a holographic dual to a 2+1 system that undergoes a superconducting phase transition. We study the electrical conductivity and spectral density of an isotropic superconducting phase. We show that the theory exhibits a pseudogap at low temperatures and a nonzero Hall conductivity. The Hall conductivity is possible because of spontaneous breaking of time reversal symmetry.

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 20

Time-reversal symmetry breaking in underdoped cuprates

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 21

Experimental observation of the polar Kerr effect in underdoped cuprates YBa2Cu3O6+x

Observation of the polar Kerr effect demonstrates spontaneous time-reversal-symmetry breaking (TRSB) in underdoped cuprates.

TRSB is unrelated to superconductivity.

TRSB represents a different phase transition, which seems to be related to the pseudogap.Xia, ..., Kapitulnik,

PRL 100, 127002 (2008)

Quantum magnetic oscillations

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 22

More evidence for a phase transition line

Kapitulnik et al., New J Phys 11, 055060 (2009)

More evidence for the time-reversal symmetry breaking at “pseudogap” line ▪µSR: Sonier et al., Science 292, 1692

(2001) ▪Neutron scattering experiments: Fauqué et al., PRL 96, 197001 (2006) Mook et al., PRB 78, 020506 (2008) ▪Noise dynamics: Van Harlingen, PRL

104, 177001 (2010)

Telegraph noise develops below the “pseudogap” line. Domain motion? Domains imply symmetry breaking due to a phase transition. The noise is sensitive to a magnetic field. TRSB?

Growing experimental evidence shows that the “pseudogap” line is a phase transition line with symmetry breaking.

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 23

Pseudogap transition in Bi2201 in ARPES, Kerr effect, and time-resolved reflectivity

Science 331, 1579 (2011)

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Initial interpretation:Kerr effect = macroscopic TRSB

The dxy+idx2

–y2 density wave model

• breaks macroscopic time-reversal symmetry• has non-zero Berry curvature• exhibits anomalous (sponaneous) Hall effect with σxy≠0• shows polar Kerr effect with θK≠0

Theoretical scenario by Tewari, Zhang, Yakovenko, & Das Sarma, PRL 100, 217004 (2008), based on Yakovenko, PRL 65, 251 (1990):

dxy+idx2

–y2 density wave with Q=(1/2,1/2)

24

idx2

–y2 density wave:

staggered currents along bonds

dxy+idx2

–y2

density wave:modulation of plaquettes

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 25

SdH magnetic oscillations, pockets, and the idx2

–y2 density wave

Observation of the Shubnikov-de Haas quantum magnetic oscillations in the underdoped cuprates can be most naturally explained by formation of small pockets on the Fermi surface.

The pockets can be produced by a superstructure with the wave vector Q=(π,π), which doubles the unit cell of the crystal.

The superstructure may originate from fluctuating antiferromagnetism or SDW.

However, there is another possibility: formation of the d-density wave.

�

i ψ + x + a,y( )ψ x,y( ) −ψ + x,y( )ψ x + a,y( ) ≠ 0

= −i ψ + x,y + b( )ψ x,y( ) −ψ + x,y( )ψ x,y + b( ) ≠ 0

(π,π)

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 26

idx2–y

2 density wave: staggering currentsIn real space, the idx

2–y

2 density wave represents staggering currents along the bonds of the lattice.

Strictly speaking, it is not a density-wave, because the electron density is not modulated, only the current is. All sites of the lattice remain equivalent. Thus, it may be difficult to detect directly.

The d-density wave was first proposed by Halperin and Rice in 1960s.

For cuprates, it was discussed in 1980s and 1990s by many people. In 2000s, it was advocated for cuprates by Chakravarty et al.

The staggering flux breaks the micro time-reversal symmetry, but not macro, because the combined symmetry with translation is preserved. Thus, idx

2–y

2 density wave alone is not enough to explain the Kerr effect.

The idx2

–y2 density wave correspond to the following electron-hole pairing:

( )† 2, cos cos2 x yiW W k kψ ψ+

Δ∝ = −k Q k k k

�

Q = π ,π( )

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 27

The chiral dxy+idx2–y

2 density wave

The dxy density wave represents staggering modulation of the diagonal tunneling amplitudes between the next-nearest neighboring sites. It breaks the symmetry between the plaquettes. The dxy density wave may originate from an electronic instability or a structural transition.

The combined dxy+idx2

–y2 density wave breaks the

time-reversal symmetry, because it breaks the symmetry between the staggered fluxes.

Yakovenko, PRL 65, 251 (1990) calculated the intrinsic (spontaneous) quantum Hall effect for the dxy+idx

2–y

2 density wave.

Let us consider an additional dxy density wave with a small amplitude Δ1:

( )† 21, sin sin , cos cos

2x y x yV iW V k k W k kψ ψ+

Δ∝ + = Δ = −k Q k k k k k

The dxy and the idx2

–y2 transitions generally occur at different temperatures.

Acoustic anomaly around 300 K (Boebinger, Migliori, et al. March 2011) − dxy?

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 28

where n is the refraction coefficient, d is the interlayer distance.

The ac Hall conductivity σxy(ω) is given by the one-loop response functionAx Ay

A textbook formula relates the Kerr angle θK with the ac Hall conductivity σxy(ω)

Calculation of the Kerr angle

The Hamiltonian of the problem is a 2×2 matrix

The Hamiltonian has a non-zero Berry curvature when Δ1 and Δ2 are present

( ) ( )2 2 2 21 22 4 sin sin sin sinx y x y

x y

t k k k kk k

⎡ ⎤∂ ∂Ω = − ⋅ × = Δ Δ + −⎢ ⎥

∂ ∂⎢ ⎥⎣ ⎦

w wk w

�

ˆ H =εk Vk + iWk

Vk − iWk εk +Q

⎛

⎝ ⎜

⎞

⎠ ⎟ = ˆ τ ⋅ w k( ) + ˆ I w0 k( )

εk = −2t coskx + cosky( ) + 4t 'coskx cosky

�

θK = Im4πσ xy ω( )n n2 −1( )ωd

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 29

1) For ω=0, we get the dc Hall conductivity

2) For optical ω>>T, we get

The Berry curvature results in a non-zero Hall conductivity σxy(ω) in the

absence of an external magnetic field (the intrinsic or spontaneous Hall effect)

The anomalous Hall conductivity

where nF(E) is the Fermi occupation function of the upper and lower bands.

The imaginary part σ”xy(ω) represents vertical transitions across the gap 2w.

( )( )

( ) ( ) ( ){ }( ) ( ) ( )

2

2 2 22F F

xy

n E n Ed kw w w

σ ωω ωπ

+ −⎡ ⎤ ⎡ ⎤Ω −⎣ ⎦ ⎣ ⎦=⎡ ⎤ ⎡ ⎤− +⎣ ⎦ ⎣ ⎦

∫k k k

k k k

( )( )

( )( )

( ) ( ) ( )

2 2

2 3-

2

2-

042

1" 24

BZpockets

BZpockets

xy

xy

e d kh w

d k w

σπ

σ ω δ ωω π

Ω=

⎡ ⎤= Ω −⎣ ⎦

∫

∫

kk

k k

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 30

Charge-density wave with staggered currents Wang and Chubukov, PRB 90, 035149 (2014)

Anomalous Hall conductivity and Kerr effect due to• Impurities: Wang, Chubukov, Nandkishore,

PRB 90, 205130 (2014) • Berry curvature: Gradhand, Eremin, Knolle,

PRB 91, 060512 (2015)

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

New developments: Karapetyan et al. PRL 109, 147001 (2012), PRL 112, 047003 (2014)

Conclusion: not TRSB!

‣ Sign of θK cannot be trained by a magnetic field‣ Sign of θK is the same on the opposite surfaces‣ θK changes linearly with applied uniaxial strain

31

La1.875Ba0.125CuO4

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Circular dichroism due to spatial dispersion if inversion and mirror symmetries are broken (chirality or natural optical activity)

is a pseudoscalar

Proposals for Kerr effect due to chiral order without TRSB:• Arfi & Gor’kov, PRB 46, 9163 (1992): Broken inversion symmetry

• Hosur, Kapitulnik, Kivelson, Orenstein, Raghu, PRB 87, 115116 (2013): Various density-wave chiral structures

• Orenstein & Moore, PRB 87, 165110 (2013): Berry curvature

• Mineev, PRB 88, 134514 (2013): Noncentrosymmetric media with spin-orbit

• Pershoguba, Kechedzhi, & Yakovenko, PRL 111, 047005 (2013): Helical texture of loop currents

32

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Varma’s loop currents

Anapole moment

O

O

O

O

Cu

Symmetries:Time-reversal oddInversion odd

Helical structure

Chirality:

Neutron scattering (Bourges et al.) finds tilted magnetic fields with an in-plane component.

Twisted model gives the tilt due to the double-helix spiral pattern of magnetic field lines.

33

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

O

O

O

O

Cu

Magneto-electric effect in Varma’s model

Electric polarization

Magnetization

Physical Intuition: External field breaks symmetry between red and blue currents.

In-plane electric field --------- out-of-plane magnetizationOut-of-plane magnetic field --------- in-plane polarization

34

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Dielectric response in a multilayer helical structure with magnetic interlayer coupling

Consider a transverse electromagnetic wave propagating along z axis.

However, polarization on the surface layer is P0=N1(N0E1).In calculation of the Kerr effect upon reflection, the bulk and the surface contributions cancel out, so the Kerr effect vanishes!

35

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

By Onsager’s reciprocity principle, reflection matrix is symmetric for a time-reversal system, so the Kerr effect must vanish and cannot be obtained due to chiral order

• Bert Halperin, High-Tc Proceedings (1992) • Peter Armitage, PRB 90, 035135 (2014)• Alex Fried, PRB 90, 121112 (2014)

Retractions of claims for Kerr effect due to chiral order• Mineev and Yoshioka, PRB 89, 139902 (2014)• Hosur, Kapitulnik, Kivelson, Orenstein, Raghu, Cho, Fried, PRB 91, 039908 (2015)

• Pershoguba, Kechedzhi, and Yakovenko, PRL 113, 129901 (2014)Different forms of constituent relations with surface terms:

- incorrect- incorrect

- correct, zero Kerr effect

36

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

“Multipole Theory in Electromagnetism” by R. E. Raab and O. L. de Lange (Oxford University Press, 2005)

37

The primed functions are odd with respect to time reversal

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Microscopic TRSB & Kerr effect in antiferromagnets

Magnetoelectric effect in Cr2O3F = c1EzBz + c2(ExBx+EyBy)

predicted by Dzyaloshinskii Sov. Phys. JETP 10, 628 (1960)observed by Astrov Sov. Phys. JETP 11, 708 (1960)

Dzyaloshinskii Phys Lett A 155, 62 (1991)

Cr2O3

Kerr effect in Cr2O3predicted by Hornreich and Shtrikman, PR 171, 1065 (1968)observed by Krichevtsov et al. J Phys Cond Mat 5, 8233 (1993)

‣ Same sign of the Kerr effect on the opposite surfaces‣ Magnetoelectric training by applying E and B

38

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 39

Measurements of the Kerr effect in Cr2O3

Krichevtsov et al. J Phys Cond Mat 5, 8233 (1993)

Krichevtsov et al. PRL 76, 4628 (1996)

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Tilted loop current models for cuprates

Weber et al. PRL 102, 017005 (2009) gives θK=0, no Kerr effect

Orenstein, PRL 107, 067002 (2011) θK≠0 but disagrees with neutrons

Yakovenko Physica B (2015)Yuan Li, PhD thesis 2010θK≠0, agrees with neutrons

40

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 41

Emergent loop current (LC) order from pair density wave (PDW) superconductivityAgterberg et al. PRB 91, 054502 (2015)

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko

Experimental proposals

Nonlinear Hall effect [Gao, Yang, Niu, PRL 112, 166601 (2014)]

O

O

O

O

Cu

In Varma’s model, an in-plane electric field E induces an out-of-plane magnetic field

E and Beff produce an in-plane Hall current

Possible experimental manifestations:

(1) dc Hall current proportional to the intensity of ac radiation:

(2) Second harmonic generation:

Permitted because Varma’s model breaks inversion and time reversal

EjH

Magnetic-field-induced polarity to be observed by STM

42

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 43

Second harmonic generation and visualization of AFM domains in Cr2O3

Fiebig et al. J Opt Soc Am. B 22, 96 (2005)

Theories of spontaneous time-reversal symmetry breakingVictor Yakovenko 44

Summary: Yakovenko, Physica B 460, 159 (2015)The tilted loop current model for cuprates explains• Kerr effect of the same sign on the opposite surfaces• No magnetic-field training, but proposes magneto-electric one• Tilted intra-unit-cell magnetic moments observed by neutrons• Optical axes rotation away from a and b, Lubashevsky et al. PRL 112, 147001 (2014)

Not explained• The absence of local magnetic field on apical oxygen in NMR

Proposed experiments for inversion and time reversal breaking• Magnetic-field-induced polarity in STM• Nonlinear Hall effect: ‣ Second-harmonic generation‣ Photogalvanic effect, dc current proportional to ac intensity

Surprising connection with experiments in Sr2IrO4 by D. Hsieh

Recommended